Presentation on theme: "Simulations of sub-100nm strained Si MOSFETs with high- gate stacks Lianfeng Yang, Jeremy Watling *, Fikru Adamu-Lema, Asen Asenov and John Barker Device."— Presentation transcript:
Simulations of sub-100nm strained Si MOSFETs with high- gate stacks Lianfeng Yang, Jeremy Watling *, Fikru Adamu-Lema, Asen Asenov and John Barker Device Modelling Group, University of Glasgow Tel: Fax: th International Workshop on Computational Electronics (IWCE-10) 24th - 27th October 2004
Outline Introduction Device structure (Conventional and strained Si n-MOSFETs) Device Calibration High- dielectrics Results and discussion Conclusions
Introduction High- dielectrics Scaling of MOSFETs beyond the 45nm technology node expected by 2010 (ITRS), requires extremely thin SiO 2 gate oxides (~0.7nm) resulting in intolerably high gate leakage. Maximise gate capacitance: The leading contenders at present are HfO 2 and Al 2 O 3. However, there is a fundamental drawback due to the resulting mobility degradation. Strained Si Has already demonstrated significant enhancement for CMOS applications.
Gate Leakage current density due to gate tunnelling From ITRS 2003 edition
Mobility enhancement in strained Si Monte-Carlo calculation of the low-field in- and out-of-plane electron mobilities in strained Si as a function of Ge content within the SiGe buffer; inset shows the in and out-of-plane directions. Our ensemble Monte Carlo simulator includes all relevant scattering mechanisms: optical intervalley phonon, inelastic acoustic phonon, ionized impurity, along with interface roughness scattering. The simulator has been thoroughly calibrated for bulk Si transport.
Device Structure Evolution
Strained Si with high- dielectrics IBM demonstrated the high performance of strained silicon (30% enhancement) with low leakage of high- insulators (1000 lower leakage) for maximum performance with minimum standby power Intel presented their high- on strained Si technology at IEDM 2003 Source: IBM (VLSI 2002)
Simulation of 67nm IBM Relaxed and Strained Si n-MOSFET Comparison between n-type Strained Si and control Si MOSFETs: 67nm effective channel length Similar processing and the same doping conditions In the strained Si MOSFET: 10nm tensile strained Si layer Strained Si on relaxed SiGe (Ge content: 15%) K.Rim, et. al., Symposium on VLSI Technology 2001
Strained Si n-channel MOSFET Structure Comparison between the n-type Strained Si and control Si MOSFETs: 67nm effective channel length Similar processing and doping conditions Oxide thickness, t ox =2.2nm (SiO 2 ) For the strained Si MOSFET: 10nm strained Si layer thickness Strained Si on relaxed SiGe (Ge content: 15%) SiGe n-MOSFET >35% drive current enhancement (70% high field mobility enhancement)
Device Calibration – Drift Diffusion Drift-diffusion (MEDICI ™ ) device simulations Concentration dependent, Caughy- Thomas and perpendicular field dependent mobility models Corrected Si/SiGe heterostructure parameters: band gap and band offsets, effective mass, DoS and permittivity † Calibrated I D -V G characteristics of the 67nm n-type bulk Si and strained Si MOSFETs (experimental data from Rim VLSI’01) † L. Yang, et al, ‘Si/SiGe Heterostructure Parameters for Device Simulations’,to Semiconductor Science and Technology 19, p (2004)
Device Calibration – Monte Carlo Calibrated I D -V G characteristics for 67nm conventional Si and strained MOSFETs, comparison with experimental data of Rim. Smoother interface for strained Si/SiO 2 interface. See L. Yang et al, Proceedings of the 5 th European Workshop on Ultimate Integration of Silicon (ULIS04), p23-26, IMEC 2004
Problems associated with high- dielectrics
High- dielectrics Fischetti, JAP’01 Scalability Leakage “Ideal” high- films: thermally stable, free from electron and interface traps, leakage- free, reliable and reproducible, etc. Replace SiO 2 Ionic polarization Electronic polarization 1/E g High- dielectrics: High dielectric constant Small bandgap Highly polarized “soft” metal-oxygen bonds which screen external fields low energy lattice oscillation (soft - phonon energy) Quantity/DielectricSiO 2 Al 2 O 3 HfO 2 oo ∞∞ TO1 (meV) TO2 (meV) SO1 (meV) SO2 (meV)
Coupling strength between the inversion layer electrons and the soft optical (SO) phonons (from the LO modes of insulator) Fröhlich interaction Ionic polarization Electronic polarization Static Optical (high frequency) SiO 2 – small difference between and High- – large difference between and Strong SO phonon scattering degrades the inversion layer carrier mobility within the MOSFET with high- gate stacks. Remote (SO) Phonon Scattering
Monte Carlo simulations of Si MOSFET with HfO 2 I D -V G characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering from the HfO 2 oxide.
Monte Carlo simulations of strained Si MOSFET with HfO 2 I D -V G characteristics of 67nm n-type strained Si MOSFET with and without soft-optical phonon scattering from the HfO 2 oxide.
Observations We observe that those simulations which include soft- optical phonon scattering exhibit a similar percentage reduction for both Si and strained Si n-MOSFETs at the same gate over drive V G -V T = 1.0V. The degradation in the drive current is ~40-50% at V D =0.1V and ~25% at V D =1.2V. SO phonon scattering decreases at high-drain voltages as the ‘Fröhlich’ interaction decreases with energy.
Velocity profile along the channel Average channel velocities for the 67nm n-type bulk and strained Si MOSFETs, with and without soft-optical phonon scattering from the HfO 2 gate stack.
Monte Carlo simulations of Si MOSFET, with Al 2 O 3 I D -V G characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering, from the Al 2 O 3 oxide.
Impact of high- on Strained Si Source: Intel, IEDM 2003
Conclusions We have investigated the impact on the performance degradation in sub 100nm n-MOSFETs due to soft-optical phonon scattering in the presence of high- dielectrics HfO 2 and Al 2 O 3. A device current degradation of around 25% at V G -V T =1.0V and V D =1.2V is observed for conventional and strained Si devices with a 2.2nm EOT HfO 2. Correspondingly a current degradation of around 10% is observed for conventional and strained Si devices with a 2.2nm EOT Al 2 O 3. Our results indicate that the performance degradation associated with high- gate stack MOSFETs can be compensated by the introduction of strained Si channels. The infancy of high- gate fabrication techniques means that overall performance degradation associated with high- gate dielectrics is expected to be worse than the predictions here.